Substitution studies of Mn and Fe in Ln6W4Al43 (Ln=Gd, Yb) and the structure of Yb6Ti4Al43
Treadwell, LaRico J.; Watkins-Curry, Pilanda; McAlpin, Jacob D.; Prestigiacomo, Joseph; Stadler, Shane; Chan, Julia Y.; Journal of Solid State Chemistry 210 (2014) 267–274; doi:10.1016/j.jssc.2013.11.021

data_1562489
_publ_section_title
;
 Substitution studies of Mn and Fe in Ln6W4Al43 (Ln=Gd, Yb) and the
 structure of Yb6Ti4Al43
;
_journal_issue                   1
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              267
_journal_page_last               274
_journal_paper_doi               10.1016/j.jssc.2013.11.021
_journal_volume                  210
_journal_year                    2014
_chemical_formula_moiety         'Al41.76 Fe1.24 W4 Yb6'
_chemical_formula_sum            'Al41.76 Fe1.24 W4 Yb6'
_chemical_formula_weight         2969.58
_space_group_IT_number           193
_space_group_name_Hall           '-P 6c 2'
_space_group_name_H-M_alt        'P 63/m c m'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   10.971(3)
_cell_length_b                   10.971(3)
_cell_length_c                   17.612(5)
_cell_measurement_reflns_used    2212
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      32.03
_cell_measurement_theta_min      2.55
_cell_volume                     1835.8(9)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device       'Nonius KappaCCD'
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0187
_diffrn_reflns_av_sigmaI/netI    0.0163
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            4000
_diffrn_reflns_theta_full        32.03
_diffrn_reflns_theta_max         32.03
_diffrn_reflns_theta_min         3.15
_exptl_absorpt_coefficient_mu    29.076
_exptl_absorpt_correction_T_max  0.3832
_exptl_absorpt_correction_T_min  0.3832
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL Scalepack (Otwinowski & Minor 1997)'
_exptl_crystal_colour            Silver
_exptl_crystal_density_diffrn    5.372
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Fragment
_exptl_crystal_F_000             2582
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.295
_refine_diff_density_min         -1.337
_refine_diff_density_rms         0.279
_refine_ls_extinction_coef       0.00059(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.219
_refine_ls_matrix_type           full
_refine_ls_number_parameters     54
_refine_ls_number_reflns         1191
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.219
_refine_ls_R_factor_all          0.0207
_refine_ls_R_factor_gt           0.0196
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0163P)^2^+15.2874P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0452
_refine_ls_wR_factor_ref         0.0456
_reflns_number_gt                1160
_reflns_number_total             1191
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            JSSC-2014-210-267.cif
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Hexagonal' was changed to
'hexagonal' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_cell_volume        1835.8(8)
_cod_database_code               1562489